(the following subsection was adapted from “Formation of DNA-copolymer fibrils through an amyloid-like nucleation polymerization mechanism” by Dawid Kedracki, Sergey K. Fillipov, Nidhi Gour, Helmut Schlaad and Corinne Nardin, Macrolomolecular Rapid Communications-DOI 10.1002/marc.201400728, Supporting Information with the figures mentioned in the text are placed at the end of this subsection)
ABSTRACT. Conjugation of a hydrophobic poly(2-oxazoline) bearing tertiary amide groups along its backbone with a short single stranded nucleotide sequence results in an amphiphilic comb/graft copolymer which organizes in fibrils upon direct dissolution in water. Supported by CD, AFM, TEM, and scattering data, fibrils are formed through inter- and intra-molecular hydrogen bonding between hydrogen accepting amide groups along the polymer backbone and hydrogen donating nucleic acid grafts leading to the formation of β-sheet layers which close into hollow tubes.
Soft materials based on self-assembling copolymers hold great promises for applications in the biomedical field as well as for the development of future technologies based on the design of advanced functional materials resulting from their hierarchical organization at several length scales . Self-assembling copolymers organize into sophisticated functional structures through non-covalent interactions such as hydrophobic, electrostatic, π-π stacking and hydrogen bonding . Bio-inspired polymers belong to a particular class of polymers which form such subtle superstructures through non-covalent interactions . Moreover, coupling of biological components with synthetic polymers could greatly improve the biocompatibility of the resulting material. Such block copolymers are referred to as
bioconjugates”, biohybrids”, or “macromolecular chimeras” . Molecular chimeras are constitutive of the first class of compounds combining the suitable properties of synthetic polymers such as protein repellency, temperature sensitivity with the features of biological molecules (e.g. targeting-antibodies) . Biopolymer assemblies are thus obviously attractive for healthcare and pharmaceutical applications. Nevertheless, the selection of the biological segment is not restricted to one class of molecules and it could be either an amino acid chain (peptide) or nucleic acid chain (DNA, RNA) as well as an oligo- or a polysaccharide.
Molecular chimeras in which the biological component is a single stranded DNA fragment belong to a particularly interesting class. Owing to DNA involvement in a plethora of vital biological mechanisms in addition to the transfer of the universal genetic information, the conjugation of DNA with biocompatible polymers has recently become a subject of intensive studies [222-224]. Conjugation is for instance expected to overcome issues such as limited plasma half-life as well as cellular penetrability [225, 226]. Besides, coupling with non-water soluble synthetic polymers results in the formation of self-assembled structures revealing the remarkable properties of the constitutive DNA fragment [113, 227-230].
An intriguing synthetic polymer species is poly(2-alkyl-2-oxazoline) (POX), which due to their structural resemblance to polypeptides are also regarded as pseudopeptides . In comparison to amino acid sequences, poly(2-oxazoline)s contain tertiary amide groups without any chirality center (or tacticity) that may disturb or prevent the formation of higher order structures. However, chirality as well as control over polymer hydrophobicity can be easily achieved through modification with side chain substituents, which further opens the opportunity for construction of complex and hierarchical biomimetic self-assemblies .
Generally, self-assembly occurs due to microphase separation of chemically distinct blocks into nanoscale periodic domains  in which segregation of chemically unlike blocks as well as cohesive interactions of like blocks can be considered as the driving force . Self-assembly of amphiphilic molecules in aqueous solution can thus be defined as a process of seeking for the delicate equilibrium between the attractive and repulsive intermolecular interactions.
The synthesis of β-sheet-mimicking copolymers is of high interest as well to both develop new classes of materials for biomedical applications and to understand the basic rules of nanoscale assembly . Reports provided up to date describe block copolymers composed of either peptide sequences able to form β-sheets or cyclic peptides forming fibrillar superstructures or nanotubes in aqueous solutions [110, 203, 231]. This self-assembly has drawn much attention because of its association with neurodegenerative diseases such as Alzheimer’s, Parkinson’s, Huntington’s diseases, type II diabetes or Creutzfeldt-Jacob disease [232, 233]. The accumulation of misfolded protein aggregates called amyloid fibers is the typical hallmark of these diseases. These amyloid fibril formation proceeds by a nucleation dependent polymerization process seeded by initial globular structures which assemble into protofilaments and bundles of twisted β-sheets .
Herein we report the self-assembly behavior of an amphiphilic POX-graft-DNA copolymer, obtained by solid phase coupling between the poly[2-(3-butenyl)-2-oxazoline] backbone carrying N-protected amino acid side chains and a water soluble (DNA) nucleotide sequence.
Structure formation results from inter- and/or intra-molecular hydrogen bonding. To the best of our knowledge this is the first report in which self-assembly formation of a hybrid composed of a pseudo peptide and a DNA sequence occurs through a nucleation polymerization mechanism. Structures assembled in aqueous solution were characterized by circular dichroism (CD) spectroscopy, transmission and scanning electron microscopy (TEM
and SEM), atomic force microscopy (AFM) as well as small-angle X-ray scattering experiments (SAXS).
121 2. EXPERIMENTAL SECTION
Poly[2-(3-butenyl)-2-oxazoline] (POX) was obtained by cationic ring-opening isomerization polymerization of 2-(3-butenyl)-2-oxazoline as reported earlier. The isolated PBOX chains had an average length of 43 repeat units, corresponding to a number-average molar mass (Mn) of 5380 g mol-1, by 1H NMR end group analysis and a dispersity index (Mw/Mn) of 1.05 (SEC). The alkenyl groups of POX were modified with N-(tert-butyloxycarbonyl)-L -cysteine (BocCys) (Merck) by thio-click chemistry . As revealed by 1H NMR analysis (Figure S1) of the purified product POX/BocCys, 76% of the unsaturated units were functionalized with the N-protected amino acid (~33 units per chain) and 24% remained unreacted (~10 units) (chemical structure in Scheme S1 (top left)). The POX-graft-DNA polymer hybrid was obtained by solid phase synthesis following synthetic strategies reported earlier [111, 193, 234]. Briefly, a 12 nucleotide-long sequence (CTCTCTCTCTTT-3’, 5’-(CT)5T2-3’), modified with an amino group through an hexyl spacer at the 5’-end and bound to the controlled pore glass (CpG) phosphoramidite solid support at the 3’-end (Scheme S1) was reacted with the carboxylic acid group of the POX/BocCys activated by N,N'-diisopropylcarbodiimide (DIC). After the coupling reaction, the resin was washed thoroughly with DCM and DMF, filtered out prior to cleavage with liquid ammonia. The copolymer was purified by dialysis against water for 5 days (molecular weight cut-off 7500 Da) and finally freeze-dried.
122 Analytical Instrumentation and Methods
1H NMR measurements were carried out at room temperature using a Bruker DPX-400 spectrometer operating at 400.1 MHz. UV/vis absorption spectra were recorded on a Lambda 25spectrometer (Perkin Elmer, Singapore) in a quartz cuvette of 1 mm path length. The FTIR spectra were taken on a Spectrum One, Perkin Elmer instrument; samples were measured in solid state using a Single Reflection Diamond ATR. CD measurements were carried out on a JASCO J-815 spectrometer (Sand Diego, USA). Preliminary synchrotron SAXS experiments were performed on the BM26B beam line (ESRF, Grenoble, France) using a pixel detector (1M PILATUS). The X-ray scattering images were recorded using a monochromatic incident X-ray beam (λ = 0.154 nm) covering the 0.023 nm-1 < q < 1.65 nm-1 range of momentum transfer (q = 4π/λ sinθ), with 2θ the scattering angle). Further measurements were performed on the B21 beam line (Diamond Light Sourse, Didcot, UK) in the 0.025 nm-1 < q < 4.00 nm-1 range. In all cases reported in here, the two-dimensional scattering patterns were isotropic.
They were azimuthally averaged to yield the dependence of the scattered intensity Is(q) on the momentum transfer q. Prior to fitting analysis, the solvent scattering has been subtracted. All data manipulations were performed using the BH plot and Data Tools software implemented in SAXS utilities. For SAXS measurements the POX-graft-DNA copolymer was dissolved in water at neutral pH to obtain the final concentration of 1mg mL-1. Subsequently the sample was vortexed thoroughly and left for equilibration at least for 24 h. Prior to transmission electron microscopy (TEM) imaging, 400-mesh copper grids were glow discharged for 30 s to render the grids surface more hydrophilic. TEM images were recorded on a Tecnai G2 electron microscope (Tokyo, Japan) operating at 120 kV. 5 µL of sample (1 mg mL-1) was deposited on a carbon coated 400-mesh copper grid and after 30s of adsorption liquid was blot off on filter paper by holding it vertically. After preparation, the sample was imaged without staining. AFM images were acquired using an MFP-3D microscope (Asylum Research, Santa
Barbara, CA) in the non-contact mode at room temperature. For all AFM measurements, cantilevers (Pointprobe NSC, MikroMasch, Tallin, Estonia) with an elastic constant of Kc = 4.28 Nm-1, and resonance frequency of 137 kHz were used. SEM images were acquired on a Jeol 6510LV microscope (München, Germany), equipped with a tungsten filament gun, operating at 10.6 mm WD and 10 kV.
3. RESULTS AND DISCUSSION
POX-graft-DNA is an amphiphilic copolymer with the chemical structure shown in Scheme 4-1. Analysis by analytical ultracentrifugation (AUC) sedimentation-velocity (Figure S2) reveals distinct sedimentation profiles of the starting materials and the final product which supports the success of the solid phase synthesis route (see Experimental Section). Estimation of the grafting density by UV/vis spectroscopy  (Figure S3) indicates that every polymer chain carries in average one DNA graft, hence POX-graft-DNA is a actually an AAB hetero three-arm star polymer with a molar mass of ~16.3 kDa and hydrophilic weight fraction of 67%.
The CD spectrum of the pristine nucleic acid sequence is displayed in Figure S4. The positive large wavelength band at λ = 280 nm and negative Cotton effect at about λ = 245 nm is characteristic of the DNA B-form . Comparing with the spectrum of POX-graft-DNA, the characteristic minimum of β-sheet structures appears at λ = 218 nm . It can be concluded that conjugation of the polymer and the nucleotide sequence and subsequent dissolution in aqueous solution results in the formation of a structure of higher order.
124 Scheme 4-1. Chemical structure of POX-graft-DNA
Direct dissolution of the final product in water at a concentration of 1 mg mL-1 results indeed in the formation of large structures due to both chemical and physical incompatibility between the non-water soluble polymer segment and the hydrophilic nucleic acid grafts.
Morphological characterizations performed by atomic force microscopy (AFM) revealed the presence of spherical aggregates of (1.8±0.4) µm average diameter (Figure S5A and S5B) along with fibrillar structures of (1.60±0.30) µm diameter and length in the range of few tens of microns (Figure 4-6 A). Cross-sectional analysis (Figure S5C) allowed obtaining information about the height of the aggregates which is of about (184±50) nm. The difference between diameter and height suggests that fibers probably collapsed upon interaction with the surface and shrinkage occurs by measurement in the dry state, which could be an indication of their hollowness. Due to presence of the electron dense phosphate groups along the nucleotide sequence, which are natural enhancers of the contrast in transmission electron microscopy (TEM) imaging could be conducted without staining. TEM revealed the presence of tubular structures with a light inner core and dark periphery which could indicate that POX-graft-DNA copolymers compose the walls of hollow fibrils (Figure 4-6 B).
Figure 4-6. Fibers morphology assembled by that POX-graft-DNA as assessed by A) AFM and B) TEM imaging
SEM imaging could however be conducted at different time intervals after product dissolution to provide information about the kinetics of fibers formation. Imaging conducted within hours (Figure 4-7 A) after dissolution reveals the formation of globular structures and protofibers which over tens of hours aggregated (Figure 4-7 B) to form highly organized filaments (Figure 4-7 C). Such as behavior is comparable to the process of nucleation polymerization characteristic of the formation of polypeptide fibrillar structures . Initial globular structures, assembled owing to the chemical incompatibility between the polymer and the nucleic acid sequence, might play the role of seeds for the fibrillation process to occur [203, 236]. According to research outcomes reported by Hamley and coworkers, the formation of polypeptide fibrils arises from co-action between polypeptide backbones, while folding occurs as a result of highly specific interaction of the side chains. Since the fibril length is related to the rate of aggregation, the significant dimensions of fully formed fibers could be due to the slow process of aggregation.
Figure 4-7.SEM imaging A) initial state-globular and protofibers structures B) intermediate aggregation C) fully formed fibers
To examine the impact of hydrogen bonding in the process of structure formation, POX-graft-DNA fibers were co-incubated with urea which is inhibiting hydrogen bonding. In the presence of 0.1 M urea fibers were completely disorganized after 24 hours (Figure S6), which thus evidences the key role of hydrogen bonding in fibrillar structures formation.
In order to obtain more detailed information about the morphology of POX-graft-DNA fibers, characterization through small-angle X-ray scattering (SAXS) was eventually performed.
SAXS curves (Figure 4-8) could be analyzed with the form factor of a hollow cylinder of finite length in the micrometer range (8600 nm) in combination with that of a Gaussian coil.
The best possible fit was achieved with structures of 17 nm inner radius and outer radius of 76 nm, in close agreement with the results obtained by imaging.
A) B) C)
Figure 4-8. SAXS outcomes of fibers assembled by POX-graft-DNA at 1 mgmL-1 in aqueous solution
Following the reports on copolymer with structural resemblance to POX-graft-DNA [190, 221] we can hypothesize that initial globular structures are formed due to microphase separation of the incompatible blocks which are subsequently stabilized by intra- and inter-molecular hydrogen bonding between the POX tertiary amides and the nucleic acid strands involved in the structure formation through nucleation dependent polymerization . It can be assumed that chains are oriented parallel to the long axis of the microfiber and linked together via hydrogen bonding. Needless to say, intermolecular hydrogen bonding is probably determining but not the only factor for formation of this specific architecture. In addition to the role of the hydrophilic weight fraction, which drives the formation of the globular structures, intramolecular interactions might play a role. This hypothesis is supported by experimental results reported previously . The grafting of a larger number of nucleic acid sequences along the POX backbone results in the self-assembly of micelles. In that case,
intramolecular hydrogen bonding is prevented, being the self-assembly supported by chemical incompatibility and intermolecular interactions solely.
Based on these experimental results one can however conclude that the wall of the fibers is constructed of a sheet of POX-graft-DNA chains organized as schematized in Figure 4-9.
Figure 4-9.Provisional structure of hollow tube composed of PBOX-g-DNA 4. CONCLUSIONS
The direct dissolution of the POX-graft-DNA amphiphilic copolymer in water results in the formation of fibrillar structures. It is assumed that fibers are hollow tubes with cross sectional radius of ~20 nm and length of few tens of microns. Based on the slow kinetics, fibrils are formed according to a nucleation dependent polymerization mechanism. The walls of the tubes are composed of POX-graft-DNA layers formed through intra- and inter-molecular hydrogen bonding.
129 Supporting Information
Materials: Dichloromethane (DCM) (extra dry, 99.8%), N,N-dimethylformamide (DMF)
(99.8%), sodium chloride (˃99.5%), triethylamine (99%) were purchased from Acros Organics (Geel, Belgium). Acridine orange,N,N′-diisopropylocarbodiimide (˃98%), dialysis cassettes (molecular weight cut-off 7.5kDa), were supplied by Sigma Aldrich (Buchs, Switzerland). The ammonia solution 35% was purchased from Fisher Scientific SA (Wohlen, Switzerland). 5’-CTCTCTCTCTTT-3’ modified at the 5’ end througha hexyllinker by an amino group and 5’-FITC labelled complementary DNA sequence 5’-AAAGAGAGAGAG-3’
were purchased from Microsynth Laboratory (Balgash, Switzerland). Silicon wafers single side polished, orientation N/Phos< 100 >, (625±25) μm thickness, 1-50 Ohm cm resistivity were purchased from Silchem (Freiburg, Germany). DMSO
Synthesis and characterization:
In brief, N,N′-diisopropylocarbodiimide was used to activate the carboxylic group of Boc-cysteine modified poly[2-(3-butenyl)-2-oxazoline] according to a protocol reported earlier.
The activated ester was exposed to a nucleophilic attack at the free 5‘-amino group of a 12-mer (sequence 5’-CTCTCTCTCTTT-3’) modified at the 5’ end by an amine group through a hexyl C6 linker whereas the 3’ end remains bound to the controlled pore glass (CPG) solid support. Solid phase synthesis was selected in order to avoid tedious steps of chemistry or purification. Treatment with liquid ammonia enabled to cleave the product from the resin and remove protecting groups. The final product was characterised by UV/VIS spectroscopy, and analytical ultracentrifugation.
Conjugation of amino modified DNA to N-Boc-cysteine modified poly[2-(3-butenyl)-2-oxazoline]. Poly[2-(3-butenyl)-2-oxazoline)modified with boc-cysteine (2 μmol, 25.8 mg, 1 eq), was dissolved in 1.5 mL of dry DCM and placed in a 2 mL reactor. Subsequently 11.3 μL of DIC (68 μmol, 8.5 mg, 1 eq-in respect to the number of PBOX side chains modified with cystein) was added. Later on, the reactor was mounted on a mechanical shaker for 1h at room temperature, 250 mg of solid cpg-resin bound 5’-CTCTCTCTCTTT -3’ modified at the 5’ end with an amine group through a C6 amino linker (10 µmol, 250 mg, 5 eq) was appended together with 40 µL of triethylamine. Closedreactor was shaked at room temperature overnight. Filtration is possible due to the filter located at the bottom of the reactor. All residual solution was thus removed from the reactor and the resin washed thoroughly with DCM and DMF and subsequently again with DCM to get rid off any unreacted species and other side products using syringe pressure filtration. Finally the resin was dried in presence of nitrogen and weighed in an eppendorf tube.
Removal of the cpg solid support. In order to cleave the product from the resin, beads were transferred together with 1.5 mL ofammonia solution. Mixture was kept in a thermoshaker at 40 oC for 24 h. Afterwards the resin was separated from solution. Subsequently, in order to remove unreacted species, salts and protecting groups this solution contaning product was transferred to a dialysis membrane (7500 MWCO, against milli-Q water for 5 days).
Subsequently the solution was filtered through 0.45 micron filter membranes and lyophilized.
Yield 8 mg (31% reaction yield). The resulting compound was characterised by UV-VIS AUC, and FTIR.
UV-Vis grafting density estimation.To find out the grafting density of DNA along the PBOX chain, UV-Vis spetroscopy was used as reported earlier.
Poly(oxazoline)absorbance at 260 nm is negligible, which enables this estimation. In order to
estimate the number of DNA strands per PBOX chain, the calibration curve with various concentration of 5’-(CT)5T2-3’ was established (Figure S3).
Scheme S1. Synthesis of PBOX-g-DNA
Figure S1.1H-NMR spectrum (400.1 MHz, CDCl3, r.t.) of the PBOX/BocCys precursor
Figure S2.AUC sedimation coefficient distributions of PBOX/BocCys (□), DNA (○), and
Figure S3. Absorbance calibration curve of the DNAat 260 nm.
For a representative quantification of the grafting density: absorbance value at 260;
Thus, concentration is equal to;
x= (0.101-0.0353)/0.0022= 29.9µg mL-1
Concentration for measurement;0.1 mgmL-1, volume; 1mL mDNA=29.9µg
Figure S4.CD spectrum of DNA (dashed line) and PBOX-g-DNA (solid line)
Figure S5. A) AFM imaging of initial globular structure and B) corresponding cross-sectional analysis, C) Fiber cross-sectional analysis
200 220 240 260 280 300
-10 -5 0 5 10 15
Figure S6.Imagingof fibers incubated with 0.1 M urea. A)TEM B)SEM shows disruption of fibrils.